The Reversible α →β Phase Transition of Cu2As2O7
Weil, Matthias; Lengauer, Christian; Füglein, Ekkehard; Baran, Enrique J.; Crystal Growth & Design 4 (2004) 1229–; doi:10.1021/cg049782o

data_4505378
_publ_section_title
;
 The Reversible \a \\rightarrow \b Phase Transition of Cu2As2O7
;
_journal_issue                   6
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              1229
_journal_paper_doi               10.1021/cg049782o
_journal_volume                  4
_journal_year                    2004
_chemical_formula_moiety         'Cu2 As2 O7'
_chemical_formula_sum            'As2 Cu2 O7'
_chemical_formula_weight         388.92
_chemical_name_common            'beta-copper arsenate'
_chemical_name_systematic        'beta-copper(II) pyroarsenate'
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90.0
_cell_angle_beta                 110.206(4)
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   7.0987(3)
_cell_length_b                   8.2777(4)
_cell_length_c                   4.8666(2)
_cell_measurement_temperature    673(5)
_cell_volume                     268.37(2)
_computing_cell_refinement       'Philips Pc-Riet Plus'
_computing_data_collection       'Philips Data Collector'
_computing_structure_refinement  'Philips Pc-Riet Plus'
_diffrn_ambient_temperature      673(5)
_diffrn_detector                 'position sensitive'
_diffrn_detector_type            Raytech
_diffrn_measurement_device_type  'Philips MPD'
_diffrn_radiation_monochromator  Hybrid-Monochromator
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54056
_diffrn_source                   CuK\a
_diffrn_source_target            Cu
_exptl_absorpt_coefficient_mu    23.585
_exptl_absorpt_correction_type   none
_exptl_crystal_density_diffrn    4.813
_exptl_crystal_density_method    'not measured'
_pd_block_diffractogram_id       WEI19
_pd_instr_location
' Institut fuer Mineralogie und Kristallographie, Universitaet Wien'
_pd_meas_2theta_range_inc        70.037
_pd_meas_2theta_range_max        80.021
_pd_meas_2theta_range_min        9.995
_pd_meas_number_of_points        6367
_pd_meas_scan_method             cont
_pd_proc_2theta_range_inc        0.011
_pd_proc_2theta_range_max        80.021
_pd_proc_2theta_range_min        9.995
_pd_proc_ls_background_function  'points are set manually'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     'Pseudo Voigt'
_pd_proc_ls_prof_R_factor        0.141
_pd_proc_ls_prof_wR_expected     0.110
_pd_proc_ls_prof_wR_factor       0.184
_pd_proc_wavelength              1.54056
_pd_spec_mounting                'horizontal capillary, 0.3mm diameter'
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_refine_ls_matrix_type           Newton
_refine_ls_number_constraints    0
_refine_ls_number_parameters     33
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            0.106
_refine_ls_weighting_details     'w = 1/y'
_refine_ls_weighting_scheme      calc
_cod_data_source_file            cg049782osi20040706_123518.cif
_cod_data_source_block           CuAsbeta
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value '1/y' was changed to 'calc'. New
tag '_refine_ls_weighting_details' was created. The value of the new
tag was set to 'w = 1/y'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4505378